Effect of tool offset and tilt angle on weld strength of butt joint friction stir welded specimens of aa2024 aluminum alloy welded to commercial pure cupper
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol.3 No.4, 201349Effect of tool offset and tilt angle on weld strength of butt jointfriction stir welded specimens of AA2024 aluminum alloy welded tocommercial pure cupperMoneer H. Tolephih1Hatem M. Mahmood2*Athra`a H. Hashem3Esam T. Abdullah41. University of Karbala`a, Karbala`a, Iraq2. Technical College-Baghdad, Za`afaranya, Baghdad, Iraq3. Institute of Technology-Baghdad, Za`afaranya, Baghdad, Iraq4. Technical College-Baghdad, Za`afaranya, Baghdad, Iraq* E-mail of the corresponding author: email@example.comAbstractThe aim of the present work is to investigate the mechanical properties and microstructure of butt joints friction stirwelded (FSW) of dissimilar material specimens welded with single pass .The material used is AA2024 aluminumalloy 5 mm thick and pure commercial copper .20 mm Flat shoulder tool 6 mm Pin diameter with a rotational speedof 900 rpm and 25 mm/min feed is used in this work ,the tool is tilted 2oto the Z axes of the machine. The weldedspecimens have been tensile tested at room temperature in order to analyze the mechanical properties with respect tothe parent metals. The microstructure of the welded specimens has been studied by employing optical microscopy.Micro-hardness examination is also performed on the welded specimens. FSW specimens welded with flat shouldertool and 2otilt angle showed higher ultimate stress than the specimens welded with flat shoulder tool and zero tiltangle . Specimens welded with 1 mm pin offset showed higher strength than the specimens welded with 0.5 and 1.5mm pin offset.Keywords: Friction stir welding, subsequent passes , mechanical properties1.IntroductionFriction stir welding (FSW) is a solid state welding process invented by the Welding Institute in 1991 . It has widelyused for welding soft materials such as Al and Mg alloys since then. In FSW the rotating pin is plunged into arigidly held work piece and traversed along the joint to be welded .Welding is achieved by plastic flow offrictionally heated material from a head of the pin to behind it. Such joining process is demonstrated to avoid severedistortions and the generated residual stresses are proved particularly low, compared to the traditional weldingprocesses (Bussu & Irving 2003, Jata et al. 2000).welding of copper is usually difficult by conventional fusion welding techniques because of its high thermaldiffusivity, which is 10–100 times higher than that of steels and nickel alloys. Hence, the heat input required forwelding is much higher, resulting in quite low welding speeds (Andersson et al. 2000).The FS Welded material produces three different areas: the weld nugget, the thermo-mechanically affected zone andthe external heat affected zone. The micro-structural grain structure in the weld nugget is usually very fine and equi-axed, ensuring elevated mechanical strength and ductility (Jata et al. 2000, Charit et al. 2002).The micro-structurein the weld nugget zone to undergo a continuous dynamic recrystallization process leading to elevated mechanicalproperties (Jata & Semiatin 2000).Even that the FS Welded specimens show lower proof stress at 0.2% and limited total elongations with respect to thebase metals, the mechanical results are extremely good considering the drastic conditions to which the materials aresubjected during the Friction Stirring process (Cavaliere et al. 2006). The tensile properties of the welded joints arelower than those of the base materials (Parcellona et Al. 2006, Liu et al. 2003, Liu & Maeda et al. 2003, Liu &Fujii& Maeda 2003).This advanced technology is capable to weld aluminum alloys difficult to be welded with traditional fusiontechniques (the 2xxx series alloys show limited weldability ).Dendrite structure occurs in the fusion zone due toconventional TIG and laser welding ,leading to a drastic decrease of the mechanical behavior (Su et al. 2003).The
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol.3 No.4, 201350FSW process is a sold- state process, therefore the solidification micro-structure is absent in the welded metal andthe presence of brittle inter- dendritic and eutectic phases is avoided (Rhodes et al. 1997).In this work the mechanical properties and microstructure of AA2024-Cu butt joints friction stir welded (FSW)specimens welded with 2otilt angle 20 mm diameter flat shoulder and 6 mm pin diameter tool ,were investigated.2.Experimental workThe base metal used in the present work were AA2024 aluminum alloy plate of 5 mm thick in T3 conditions andcommercial pure Copper plate 5 mm thick.The plate was cut and machined into rectangular samples of 100X 150 mm and they were butt welded using HMTmilling machine. The longitudinal direction of FSW line was perpendicular to the rolling direction of the plates.HSS tool with pin and flat shoulder diameters of 6 mm and 20 mm respectively was used to achieve the weldment.The tool rotational speed was 900 rpm and 25 mm/min travel speed , according to optimized welding parametersdetermined so far. The tool axis was tilted by 2owith respect to Z-axis of milling machine ,see fig. 1 . Pin lengthwas 4.8 mm with multi grooves of 0.5 mm depth .The experiment was achieved by plunging the pin in the Aluminum plate and then the pin moved toward thecopper side until the pin inter the copper, pin offset represents the distance which the pin inter into the copper ,seefig.2.The parameters which we aimed to study in the present work were ,the tilt angle of the tool and pin offset. Theadvance and retreat sides were kept at the Aluminum and copper plate respectively.Two sets of experiments with 0oand 2otilt angles and 1 mm offset were achieved to evaluate the optimum toolsetup which gives higher weld strength.Three other sets of experiments using 2otilt angle (the optimum tool setup) and three pin offsets of 0.5 , 1.0 and 1.5mm were achieved to evaluate the strength of the weldment depending on the pin offset in the copper side.Tensile test have been executed at room temperature using (Zwick/Roell Z100) testing machine having a loadcapacity of 100 KN, the axial applied load was perpendicular to the weld line, the specimens having calibratedstandard dimensions .The Vickers hardness profile of the welded zone have been measured 1 mm below the top surface of the toolshoulder in a direction perpendicular to the weld line , using a Vickers indenter with 500gf load for 10 sec.3.Results and discussionFriction stir welded specimens welded with 900 rpm pin rotational speed 2otilt angle and 25 mm/min feed weretensile tested to evaluate the joint strength. Three specimens were tested for each condition ,the average value forthese three tests were recorded. Tensile test results of the base metals used in the present work are listed in table 1.The tensile test results of the welded specimens are shown in Tables.2,3.Fig. 3 .Shows the stress strain curves of the welded specimens. It is clear from the tensile test results and thatwelding with 20tilted tool gives higher strength than welding with 0otilt angle . This is due to the additionalcompression of the tool shoulder which resulting in more heat .This additional compression of tilting the tool canremove any voids or tunnels resulting from the gap existing initially between the welded plates .The percentage elongation of the welded specimens was too low compared with the elongation of the base metals,this is due to the brittle interface between the welded plates which is resulted from welding dissimilar material withdifferent physical properties.
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol.3 No.4, 201351Welding with 0.5 and 1.5 mm tool offset in the copper side of the welded specimens showed less ultimate tensilestrength compared to 1 mm tool offset which recorded an ultimate tensile stress of 248 MPa (88.57% of the copperultimate tensile strength) . The heat generated when welding with 0.5 mm tool offset was not enough to loweringthe yield strength of the cupper to match the yield strength of the aluminum so that the mechanical pond resultingwas week, while welding with 1.5 mm tool offset resulting in high temperature which in turn resulting in meltingthe aluminum plate at the weld interface resulting also in low tensile strength.The fracture of the welded specimens was brittle and always occur at the weld interface.Fig.4 . shows the micro-hardness test results for the specimens welded with 1 mm tool offset and 2otilt angle ofthe tool. This figure showed that the hardness at the weld interface and 1 mm depth in both copper and aluminumwas constant and raised compared to the copper side , while lowered in comparison to the aluminum side.Fig.5. is a magnified overview of weld interface. It can be seen that many relatively coarse pieces are spreadthrough the aluminum side of the nugget. The copper pieces are well distributed within the nugget .In fig. 6 . the onion rings were clear it is known that FSW nugget of dissimilar alloys such as Al alloy welded tocopper are characterized by complex vortex-like and swirl-like intercalation (Murr et al. 1998, Murr & Li et al.1998, Ouyang & Kovacevic 2002).Fig.7.Shows the copper hook in the weld nugget which gives the weld its strength, this hook distributed along theweld line and across the depth of the weld which is resulted from the rotation of the pin.ConclusionsFrom the results of the welded specimens of AA2024 aluminum alloy to pure copper the following conclusionswere recorded.1. Welding of AA2024 aluminum alloy to pure copper with 2otool tilt angle gives higher strength thanwelding with 0otool tilt angle.2. Fracture of the welded specimens is brittle and always occur at the weld interface.3. The nugget contains large pieces of copper distributed uniformly in addition to the copper hooks.ReferencesG. Bussu, P.E. Irving, "The role of residual stress and heat affected zone properties on fatigue crack propagation infriction stir welded 2024-T351 aluminum joints", International Journal of Fatigue 25 (2003) 77–88.K.V. Jata, K.K. Sankaran, J. Ruschau, "Friction stir welding effects on microstructure and fatigue of aluminiumalloy 7050-T7451", Metallurgical and Materials Transactions 31A (2000) 2181– 2192.C.G. Andersson, R.E. Andrews, B.G.I. Dance, M.J. Russell, E.J. Olden, R.M. Samderson," A comparison of coppercanister fabrication by the electron beam and friction stir processes", Proceedings of the 2nd InternationalSymposium “Friction Stir Welding”, Gothenburg, 2000, CD-ROM.Charit, R.S. Mishra, M.W. Mahoney, "Multi-sheet structures in 7475 aluminum by friction stir welding in concertwith post-weld superplastic forming", Scripta Materialia 47 (2002) 631–636.K.V.Jata, S.L. Semiatin, "Continuous dynamic recrystallization during friction stir welding of high strengthaluminum alloys" ,Scripta Materialia 43(8)(2000)743-749.P. Cavaliere ,R. Nobile, F.W. Panella, A. Squillace, "Mechanical and microstructural behavior of 2024-7075aluminum alloy sheets joined by friction stir welding",Int. j. of machine tool manufacture 46(2006) 588- 594.A.Parcellona, G. Buffa, L. Fratini, D. Palmeri, "On micro structural phinomena accurring in friction stir welding ofaluminum alloys", Journal of material processing technology 177(2006) 340-343
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol.3 No.4, 201352H.J.Liu,H.Fujii,M.Maeda,K.Nogi,"Tensile properties and fracture locations of friction-stir-welded joints of 2017-T351 aluminum alloy", Journal of Material Processing Technology 142 (2003) 692-696.H.J.Liu, M.Maeda, H.Fujii, K.Nogi, "Tensile properties and fracture locations of friction-stir-welded joints of 1050-H24 aluminum alloy", Journal of material science letters 22, 2003, 41-43.H.J.Liu,H.Fujii,M.Maeda,K.Nogi, "Mechanical properties of friction stir welded joints of 1050-H24 aluminumalloys", science and technology of welding and joining 2003, vol.8 , No6, 450-454.J.Q. Su, T.W. Nelson, R. Mishra, M. Mahoney, "Microstructural investigation of friction stir welded 7050-T615aluminum ", Acta Materialia 51 (2003) 713-729.C.G. Rhodes, M.W. Mahoney, W.H. Bingel, "Effect of friction stir welding on microstructure of 7075 aluminum",Scripta Materialia 36(1997)69-75.Murr, L. E., Li, Y., Trillo, E. A., Flores, R. D. and McClure, J . C. "Microstructures in friction-stir welded metals".J. Mater. Processing Mfg Sci., 1998, 7(2), 145–161.Murr, L. E., Li, Y., Flores, R. D., Trillo, E. A. and McClure, J . C. "Intercalation vortices and related microstructuralfeatures in the friction-stir welding of dissimilar metals". Mater. Res. Innovation, November 1998, 2(3), 150–163.Ouyang, J. H. and Kovacevic, R. "Materials flow and microstructure in the friction stir butt welds of the same anddissimilar aluminum alloys". J. Mater. Engng Performance, January 2002, 11(1), 51–63.Moneer H. Tolephih Professor Assis.President of University of Karbala`a, Karbala`a, Iraqplace and date of birth: Karbala`a Governorate, IraqPhD ,Mechanical Engineering, University of Technology, Baghdad, Iraq, 1998Major field of study: Applied MechanicsHatem M. MahmoodLecturer, Technical College- BaghdadPlace and date of birth:Baghdad, IraqMSc Mechanical Engineering, University of Baghdad, Baghdad, Iraq, 1985Major field of study: Applied Mechanics
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol.3 No.4, 201353Fig.1. Friction stir welding toolThe tool axis was tilted by 2owith respect to Z-axis of milling machineFig. 2. Pin offset in the copper sidepin offset represents the distance which the pin inter into the copperTable 1. Mechanical properties of base metalsTensile test results of the base metals used in the present workMech. PropertiesMaterialsUltimate tensilestress(MPa)Elongation%Al Base Metal 482 17.2Cupper base metal 280 12.2
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol.3 No.4, 201354Table 2..Mechanical properties of the welded specimens welded with 2oTool tilt angleMech.PropertiesTool offsetAverage Ultimatetensile strengthMPaAverage% elongationTilt angleDeg.0.5 mm offfset 98.5 0.08 21.0 mm offset 248 0.8 21.5 mm offset 150 0.17 2The tensile test results of the welded specimens for different tool offsets.Table.3.Mechanical properties of the welded specimens welded with 0otool tilt angleMech.PropertiesTilt angleAverage ultimatetensile strengthMPaAverage %elongationTool offset(mm)0otilt angle98.5 0.08 12otilt angle 248 0.8 1The tensile test results of the welded specimens for different tilt angles.
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol.3 No.4, 201355Fig. 3 . Stress strain curves of welded specimens welded with ,(a) 0otool tilt angle and 1 mm tool offset,(b) 2otooltilt angle and 0.5 mm tool offset,(c) 2otool tilt angle and 1 mm tool offset,(d) 2otool tilt angle and 1.5 mm tooloffset.
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol.3 No.4, 201356Fig. 4 . Vickers hardness distribution 1 mm from the weld interfaceFig.5.AA2024 aluminum - copper weld interface.
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol.3 No.4, 201357Fig.6. The onion rings in the nugget of the weld
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol.3 No.4, 201358Fig.7. Cooper hook in the weld nugget
This academic article was published by The International Institute for Science,Technology and Education (IISTE). The IISTE is a pioneer in the Open AccessPublishing service based in the U.S. and Europe. The aim of the institute isAccelerating Global Knowledge Sharing.More information about the publisher can be found in the IISTE’s homepage:http://www.iiste.orgCALL FOR PAPERSThe IISTE is currently hosting more than 30 peer-reviewed academic journals andcollaborating with academic institutions around the world. There’s no deadline forsubmission. Prospective authors of IISTE journals can find the submissioninstruction on the following page: http://www.iiste.org/Journals/The IISTE editorial team promises to the review and publish all the qualifiedsubmissions in a fast manner. All the journals articles are available online to thereaders all over the world without financial, legal, or technical barriers other thanthose inseparable from gaining access to the internet itself. Printed version of thejournals is also available upon request of readers and authors.IISTE Knowledge Sharing PartnersEBSCO, Index Copernicus, Ulrichs Periodicals Directory, JournalTOCS, PKP OpenArchives Harvester, Bielefeld Academic Search Engine, ElektronischeZeitschriftenbibliothek EZB, Open J-Gate, OCLC WorldCat, Universe DigtialLibrary , NewJour, Google Scholar